Luminescent liquid crystalline materials based on palladium(II) imine derivatives containing the 2-phenylpyridine core.
Micutz, Marin; Iliş, Monica; Staicu, Teodora; Dumitraşcu, Florea; Pasuk, Iuliana; Molard, Yann; Roisnel, Thierry; Cîrcu, Viorel; Dalton transactions (Cambridge, England : 2003) 43 (2014) 1151–1161; doi:10.1039/c3dt52137k

data_7028582
_publ_section_title
;
 Luminescent liquid crystalline materials based on palladium(II) imine
 derivatives containing the 2-phenylpyridine core.
;
_journal_issue                   3
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              1151
_journal_page_last               1161
_journal_paper_doi               10.1039/c3dt52137k
_journal_volume                  43
_journal_year                    2014
_chemical_compound_source        'synthesis as described'
_chemical_formula_moiety         'C28 H36 Cl2 N2 O2 Pt S, C H2 Cl2'
_chemical_formula_sum            'C29 H38 Cl4 N2 O2 Pt S'
_chemical_formula_weight         815.56
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.3
_audit_creation_date             2011-04-26T10:20:03-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                94.842(5)
_cell_angle_beta                 92.304(5)
_cell_angle_gamma                104.881(5)
_cell_formula_units_Z            2
_cell_length_a                   7.4355(9)
_cell_length_b                   8.2355(10)
_cell_length_c                   26.969(3)
_cell_measurement_reflns_used    6659
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      27.15
_cell_measurement_theta_min      2.84
_cell_measurement_wavelength     0.71073
_cell_volume                     1587.1(3)
_computing_cell_refinement       'Bruker APEX2 (Bruker, 2006)'
_computing_data_collection       'Bruker APEX2 (Bruker, 2006)'
_computing_data_reduction        'Bruker APEX2 (Bruker, 2006)'
_computing_molecular_graphics    'Ortep-3 for Windows (Farrugia, 1997)'
_computing_publication_material
;
           WinGX publication routines (Farrugia, 1999),
           CRYSCAL (T. Roisnel, local program)
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SIR97 (Altomare et al., 1999))'
_diffrn_ambient_temperature      150(2)
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.978
_diffrn_measured_fraction_theta_max 0.97
_diffrn_measurement_device_type  'APEXII, Bruker-AXS'
_diffrn_measurement_method       'CCD rotation images, thin slices'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0499
_diffrn_reflns_av_unetI/netI     0.0675
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       34
_diffrn_reflns_limit_l_min       -34
_diffrn_reflns_number            21012
_diffrn_reflns_theta_full        25
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         2.99
_exptl_absorpt_coefficient_mu    4.852
_exptl_absorpt_correction_T_max  0.908
_exptl_absorpt_correction_T_min  0.751
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
  [Sheldrick, G.M. (2002). SADABS Bruker AXS Inc., Madison, Wisconsin, USA]
;
_exptl_crystal_colour            'pale yellow'
_exptl_crystal_density_diffrn    1.707
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             808
_exptl_crystal_size_max          0.52
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.299
_refine_diff_density_min         -1.976
_refine_diff_density_rms         0.167
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.04
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     355
_refine_ls_number_reflns         7079
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.04
_refine_ls_R_factor_all          0.0554
_refine_ls_R_factor_gt           0.0412
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0000P)^2^+6.1116P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0688
_refine_ls_wR_factor_ref         0.0726
_reflns_number_gt                6006
_reflns_number_total             7079
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3dt52137k.txt
_cod_data_source_block           job
_cod_database_code               7028582